#------------------------------------------------------------------------------
#$Date: 2024-07-05 19:06:05 +0300 (Fri, 05 Jul 2024) $
#$Revision: 293026 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/60/7716066.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7716066
loop_
_publ_author_name
'Subintoro, Primadi J.'
'Carter, Korey P.'
_publ_section_title
;
 Structural and vibrational properties of lanthanide Lindqvist
 polyoxometalate complexes.
;
_journal_issue                   22
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9526
_journal_page_last               9539
_journal_paper_doi               10.1039/d4dt00786g
_journal_volume                  53
_journal_year                    2024
_chemical_formula_moiety         'La Na9 O68.25 W10, 1.75(O)'
_chemical_formula_sum            'La Na9 O70 W10'
_chemical_formula_weight         3304.32
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_primary     direct
_audit_creation_date             2023-12-20
_audit_creation_method
;FinalCif V134 by Daniel Kratzert, Freiburg 2024, 
https://dkratzert.de/finalcif.html
;
_audit_update_record
;
2024-02-29 deposited with the CCDC.	2024-05-06 downloaded from the CCDC.
;
_cell_angle_alpha                102.062(4)
_cell_angle_beta                 97.834(4)
_cell_angle_gamma                101.546(4)
_cell_formula_units_Z            2
_cell_length_a                   12.8892(13)
_cell_length_b                   12.9526(12)
_cell_length_c                   20.1296(19)
_cell_measurement_reflns_used    9776
_cell_measurement_temperature    100.00
_cell_measurement_theta_max      37.876
_cell_measurement_theta_min      2.417
_cell_volume                     3163.8(5)
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2016/4 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      100.00
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker D8 Venture Duo'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0839
_diffrn_reflns_av_unetI/netI     0.0352
_diffrn_reflns_Laue_measured_fraction_full 0.985
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            451041
_diffrn_reflns_point_group_measured_fraction_full 0.985
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         37.883
_diffrn_reflns_theta_min         2.340
_exptl_absorpt_coefficient_mu    18.947
_exptl_absorpt_correction_T_max  0.0422
_exptl_absorpt_correction_T_min  0.0049
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1482 before and 0.1052 after correction.
The Ratio of minimum to maximum transmission is 0.1161.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.469
_exptl_crystal_description       plank
_exptl_crystal_F_000             2912
_exptl_crystal_preparation
'Sodium tungstate in aqueous media acidified with Nitric acid followed by addition of Lanthanum Nitrate solution'
_exptl_crystal_recrystallization_method 'Slow evaporation from water'
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.1
_refine_diff_density_max         5.076
_refine_diff_density_min         -3.346
_refine_diff_density_rms         0.400
_refine_ls_extinction_coef       0.00066(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2016/4 (Sheldrick 2016)'
_refine_ls_goodness_of_fit_ref   1.200
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     830
_refine_ls_number_reflns         33973
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.200
_refine_ls_R_factor_all          0.0532
_refine_ls_R_factor_gt           0.0512
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0327P)²+55.3704P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1191
_refine_ls_wR_factor_ref         0.1202
_reflns_Friedel_coverage         0.000
_reflns_number_gt                32288
_reflns_number_total             33973
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4dt00786g2.cif
_cod_data_source_block           Complex_1
_cod_depositor_comments
'Adding full bibliography for 7716058--7716071.cif.'
_cod_database_code               7716066
_olex2_exptl_crystal_mounting_method 'Mitegen Mount'
_olex2_refinement_description
;
1. Others
 Fixed Sof: O68B(0.5) O69B(0.75) O68A(0.5) O69A(0.25)
;
_olex2_submission_special_instructions 'No special instructions were received'
_shelx_shelxl_version_number     2016/4
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.116
_shelx_estimated_absorpt_t_max   0.253
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.81306(2) 0.42419(2) 0.61724(2) 0.01581(4) Uani 1 1 d . . . . .
W2 W 0.83210(2) 0.64624(2) 0.83460(2) 0.01652(4) Uani 1 1 d . . . . .
W3 W 0.68295(2) 0.60566(2) 0.68106(2) 0.01581(4) Uani 1 1 d . . . . .
W4 W 0.95934(2) 0.46431(2) 0.77138(2) 0.01704(4) Uani 1 1 d . . . . .
W5 W 0.37111(2) 0.16217(2) 0.67298(2) 0.01673(4) Uani 1 1 d . . . . .
W6 W 0.57526(2) 0.17248(2) 0.88489(2) 0.01851(4) Uani 1 1 d . . . . .
W8 W 0.95149(2) 0.67526(2) 0.69937(2) 0.01700(4) Uani 1 1 d . . . . .
W9 W 0.55761(2) 0.04067(2) 0.72446(2) 0.01775(4) Uani 1 1 d . . . . .
W10 W 0.33558(2) 0.02321(2) 0.79334(2) 0.02280(5) Uani 1 1 d . . . . .
La1 La 0.65056(3) 0.35379(3) 0.75894(2) 0.01610(5) Uani 1 1 d . . . . .
O15 O 0.8177(4) 0.7068(4) 0.6687(3) 0.0191(7) Uani 1 1 d . . . . .
O16 O 0.9199(4) 0.5616(4) 0.6166(2) 0.0194(7) Uani 1 1 d . . . . .
O6 O 0.9510(4) 0.5751(4) 0.8485(3) 0.0189(7) Uani 1 1 d . . . . .
O10 O 0.7067(4) 0.5097(4) 0.5994(2) 0.0181(7) Uani 1 1 d . . . . .
O17 O 1.0377(4) 0.5919(4) 0.7387(3) 0.0214(8) Uani 1 1 d . . . . .
O30 O 0.4769(4) 0.2643(5) 0.9114(3) 0.0228(8) Uani 1 1 d . . . . .
O12 O 0.7243(4) 0.6913(4) 0.7765(2) 0.0185(7) Uani 1 1 d . . . . .
O14 O 0.9378(4) 0.7392(4) 0.7914(2) 0.0189(7) Uani 1 1 d . . . . .
O32 O 0.2900(4) 0.1503(5) 0.8329(3) 0.0251(9) Uani 1 1 d . . . . .
O3 O 0.7161(4) 0.3315(4) 0.6450(2) 0.0189(7) Uani 1 1 d . . . . .
O33 O 0.2791(4) 0.0430(5) 0.7049(3) 0.0231(9) Uani 1 1 d . . . . .
O24 O 0.3164(4) 0.2595(4) 0.7380(2) 0.0209(8) Uani 1 1 d . . . . .
O2 O 0.5966(4) 0.4996(4) 0.7054(2) 0.0184(7) Uani 1 1 d . . . . .
O20 O 0.4822(4) 0.2666(4) 0.6693(3) 0.0200(8) Uani 1 1 d . . . . .
O22 O 0.6656(4) 0.2807(4) 0.8654(2) 0.0185(7) Uani 1 1 d . . . . .
O26 O 0.4538(4) 0.0518(4) 0.6481(2) 0.0195(7) Uani 1 1 d . . . . .
O19 O 0.4986(4) 0.3920(4) 0.8194(3) 0.0217(8) Uani 1 1 d . . . . .
O8 O 0.9331(3) 0.3924(4) 0.6721(2) 0.0175(7) Uani 1 1 d . . . . .
O1 O 0.7371(4) 0.5313(4) 0.8436(2) 0.0205(8) Uani 1 1 d . . . . .
O28 O 0.6185(4) 0.0608(4) 0.8223(3) 0.0212(8) Uani 1 1 d . . . . .
O35 O 0.4400(4) 0.0514(4) 0.8752(3) 0.0242(9) Uani 1 1 d . . . . .
O40 O 0.7864(4) 0.1642(4) 0.3870(3) 0.0228(8) Uani 1 1 d . . . . .
O48 O 0.3158(4) 0.0586(4) 0.4642(3) 0.0226(8) Uani 1 1 d . . . . .
O42 O 0.3581(4) 0.5248(4) 0.5434(3) 0.0241(9) Uani 1 1 d . . . . .
O13 O 0.8254(4) 0.5405(4) 0.7237(2) 0.0187(7) Uani 1 1 d . . . . .
O38 O 0.4865(4) 0.3592(4) 0.5546(3) 0.0234(9) Uani 1 1 d . . . . .
O41 O 0.5818(4) 0.2687(4) 0.3039(3) 0.0237(9) Uani 1 1 d . . . . .
O31 O 0.4683(4) 0.1616(4) 0.7796(2) 0.0190(7) Uani 1 1 d . . . . .
O21 O 0.6544(4) 0.1581(4) 0.7191(2) 0.0186(7) Uani 1 1 d . . . . .
O34 O 0.4281(4) -0.0519(4) 0.7471(3) 0.0249(9) Uani 1 1 d . . . . .
O18 O 1.0431(4) 0.7766(4) 0.6795(3) 0.0229(8) Uani 1 1 d . . . . .
O51 O 0.1189(5) -0.1393(4) 0.4863(3) 0.0258(9) Uani 1 1 d . . . . .
O9 O 0.8156(4) 0.3550(4) 0.5336(3) 0.0212(8) Uani 1 1 d . . . . .
O53 O -0.0437(4) 0.0034(4) 0.3353(3) 0.0252(9) Uani 1 1 d . . . . .
O46 O 0.2399(4) 0.2881(4) 0.4738(3) 0.0223(8) Uani 1 1 d . . . . .
O49 O 0.0918(4) 0.1205(4) 0.5012(3) 0.0231(8) Uani 1 1 d . . . . .
O4 O 0.8499(4) 0.3651(4) 0.7850(3) 0.0200(8) Uani 1 1 d . . . . .
O43 O 0.3661(5) 0.4671(5) 0.6953(3) 0.0280(10) Uani 1 1 d . . . . .
O52 O 0.1841(4) 0.0781(4) 0.3244(3) 0.0242(9) Uani 1 1 d . . . . .
O62 O 0.8516(5) 0.8888(5) 1.0791(3) 0.0313(11) Uani 1 1 d . . . . .
O36 O 0.2348(5) -0.0807(6) 0.8037(3) 0.0378(15) Uani 1 1 d . . . . .
O50 O 0.1481(4) -0.1566(4) 0.3304(3) 0.0221(8) Uani 1 1 d . . . . .
O57 O 0.4598(5) 0.3832(5) 1.1503(4) 0.0341(12) Uani 1 1 d . . . . .
O5 O 0.8507(4) 0.7405(4) 0.9127(3) 0.0220(8) Uani 1 1 d . . . . .
O56 O 0.0421(5) 0.0330(4) 0.1644(3) 0.0255(9) Uani 1 1 d . . . . .
O7 O 1.0739(4) 0.4251(4) 0.8021(3) 0.0235(9) Uani 1 1 d . . . . .
O39 O 0.5672(4) 0.1794(4) 0.4410(3) 0.0228(8) Uani 1 1 d . . . . .
O66 O 0.8678(5) 0.1753(6) 1.1078(4) 0.0423(17) Uani 1 1 d . . . . .
O45 O 0.0460(5) 0.3931(5) 0.5097(3) 0.0288(10) Uani 1 1 d . . . . .
O25 O 0.2828(4) 0.1454(4) 0.5957(3) 0.0235(9) Uani 1 1 d . . . . .
O29 O 0.6374(4) 0.1646(4) 0.9656(3) 0.0246(9) Uani 1 1 d . . . . .
O27 O 0.6071(5) -0.0670(4) 0.6856(3) 0.0263(9) Uani 1 1 d . . . . .
O44 O 0.1642(5) 0.5670(5) 0.6226(3) 0.0290(10) Uani 1 1 d . . . . .
O54 O 0.1456(5) -0.1720(5) 0.1737(4) 0.0348(13) Uani 1 1 d . . . . .
O55 O -0.0932(5) -0.2117(5) 0.2241(5) 0.0415(17) Uani 1 1 d . . . . .
O47 O 0.1161(5) 0.2981(5) 0.6433(3) 0.0289(10) Uani 1 1 d . . . . .
O61 O 0.6195(5) 0.9573(5) 0.9970(3) 0.0298(11) Uani 1 1 d . . . . .
O65 O 0.6585(5) 0.7277(5) 0.9833(3) 0.0308(11) Uani 1 1 d . . . . .
O59 O 0.7331(4) 0.9066(4) 0.8518(3) 0.0249(9) Uani 1 1 d . . . . .
O23 O 0.3104(5) 0.3685(7) 0.8756(3) 0.0387(15) Uani 1 1 d . . . . .
O63 O 1.0152(6) 0.7565(7) 1.0480(3) 0.0418(16) Uani 1 1 d . . . . .
O60 O 0.9174(7) 1.0539(6) 0.9905(4) 0.0444(17) Uani 1 1 d . . . . .
O67 O 0.5641(5) 0.1755(5) 1.1130(3) 0.0319(11) Uani 1 1 d . . . . .
O70 O 0.8790(6) 0.3693(7) 1.0362(4) 0.0423(15) Uani 1 1 d . . . . .
O64 O 0.7841(7) 0.5165(7) 0.9838(4) 0.0449(17) Uani 1 1 d . . . . .
O11 O 0.5954(4) 0.6723(4) 0.6437(3) 0.0208(8) Uani 1 1 d . . . . .
O68B O 0.7022(8) 0.4289(8) 1.1310(5) 0.0220(16) Uani 0.5 1 d . . P A 1
O69B O 0.5811(9) 0.4474(9) 1.0093(6) 0.048(2) Uani 0.75 1 d . . P B 1
O58 O 0.7638(9) 0.2900(10) 1.2162(8) 0.076(3) Uani 1 1 d . . . . .
O68A O 0.7571(14) 0.3992(14) 1.1801(9) 0.051(4) Uani 0.5 1 d . . P A 2
O69A O 0.629(2) 0.3986(17) 1.0299(11) 0.028(4) Uani 0.25 1 d . . P A 2
W7 W 0.38953(2) 0.29435(2) 0.83405(2) 0.02062(5) Uani 1 1 d . . . . .
Na1 Na 0.0548(2) -0.0714(2) 0.24823(16) 0.0222(5) Uani 1 1 d . . . . .
Na2 Na 0.1229(2) -0.0103(2) 0.41263(16) 0.0235(5) Uani 1 1 d . . . . .
Na3 Na 0.4008(2) 0.2291(3) 0.44596(17) 0.0244(5) Uani 1 1 d . . . . .
Na4 Na 0.7021(2) 0.3131(2) 0.41459(16) 0.0236(5) Uani 1 1 d . . . . .
Na5 Na 0.7692(3) 0.8926(3) 0.96682(16) 0.0253(5) Uani 1 1 d . . . . .
Na6 Na 0.2268(3) 0.4050(3) 0.58618(18) 0.0301(6) Uani 1 1 d . . . . .
Na7 Na 0.6075(3) 0.3506(3) 1.2114(2) 0.0335(7) Uani 1 1 d . . . . .
Na8 Na 0.7328(3) 0.2653(4) 1.0760(2) 0.0411(9) Uani 1 1 d . . . . .
Na9 Na 0.8285(4) 0.7019(4) 1.0322(2) 0.0429(9) Uani 1 1 d . . . . .
O37 O 0.6032(4) 0.1273(4) 0.5653(3) 0.0220(8) Uani 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 W1 O13 75.09(18) . . ?
O68Ab O58 Na7 61.7(7) . . ?
O68Ab O58 Na8 58.8(7) . . ?
O10 W1 O16 83.19(19) . . ?
O10 W1 O13 76.24(18) . . ?
O3 W1 O16 160.6(2) . . ?
O3 W1 O10 90.7(2) . . ?
O3 W1 O8 92.6(2) . . ?
O3 W1 O13 85.54(19) . . ?
O8 W1 O16 85.21(19) . . ?
O8 W1 O10 154.11(19) . . ?
O8 W1 O13 78.44(18) . . ?
O9 W1 O16 95.7(2) . . ?
O9 W1 O10 101.4(2) . . ?
O9 W1 O3 103.6(2) . . ?
O9 W1 O8 102.7(2) . . ?
O9 W1 O13 170.7(2) . . ?
O68Ab Na7 O41 125.8(6) . 1_556 ?
O68Ab Na7 O43 94.0(4) . 2_667 ?
O68Ba Na7 O43 96.5(3) . 2_667 ?
O68Ab Na7 O57 116.6(6) . . ?
O68Ab Na7 O67 88.7(5) . . ?
O68Ba Na7 O67 83.1(3) . . ?
O68Ab Na7 O58 45.8(6) . . ?
O68Ba Na7 Na8 41.9(3) . . ?
O68Ab Na7 Na8 42.3(4) . . ?
O68Ba Na8 O66 130.0(4) . . ?
O68Ab Na8 O66 99.4(5) . . ?
O68Ba Na8 O29 123.0(4) . . ?
O68Ba Na8 O67 86.5(3) . . ?
O6 W2 O14 82.70(19) . . ?
O68Ab Na8 O67 85.0(5) . . ?
O68Ab Na8 O70 93.0(5) . . ?
O68Ba Na8 O70 87.5(3) . . ?
O68Ab Na8 O58 38.8(5) . . ?
O69Ab Na8 O58 115.1(6) . . ?
O68Ba Na8 O58 69.0(4) . . ?
O68Ab Na8 O69A 80.8(7) . . ?
O69Ab Na8 Na7 77.8(6) . . ?
O68Ba Na8 Na7 44.5(3) . . ?
O68Ab Na8 Na7 37.3(5) . . ?
O6 W2 O13 77.03(18) . . ?
O12 W2 O6 152.6(2) . . ?
O12 W2 O14 83.42(19) . . ?
O12 W2 O13 76.56(18) . . ?
O14 W2 O13 74.39(18) . . ?
O1 W2 O6 91.5(2) . . ?
O1 W2 O12 93.3(2) . . ?
O1 W2 O14 159.3(2) . . ?
O1 W2 O13 85.00(19) . . ?
O5 W2 O6 102.8(2) . . ?
O5 W2 O12 102.1(2) . . ?
O5 W2 O14 96.5(2) . . ?
O5 W2 O1 104.1(2) . . ?
O5 W2 O13 170.8(2) . . ?
O15 W3 O13 74.40(17) . . ?
O10 W3 O15 83.5(2) . . ?
O10 W3 O12 153.51(19) . . ?
O10 W3 O13 76.86(18) . . ?
O12 W3 O15 83.2(2) . . ?
O12 W3 O13 77.55(18) . . ?
O2 W3 O15 161.6(2) . . ?
O2 W3 O10 94.0(2) . . ?
O2 W3 O12 91.5(2) . . ?
O2 W3 O13 87.31(18) . . ?
O11 W3 O15 94.1(2) . . ?
O11 W3 O10 100.9(2) . . ?
O11 W3 O12 102.8(2) . . ?
O11 W3 O2 104.2(2) . . ?
O11 W3 O13 168.4(2) . . ?
O6 W4 O17 83.8(2) . . ?
O6 W4 O8 153.78(19) . . ?
O6 W4 O13 77.85(17) . . ?
O17 W4 O13 73.77(18) . . ?
O8 W4 O17 82.2(2) . . ?
O8 W4 O13 76.99(17) . . ?
O4 W4 O6 94.2(2) . . ?
O4 W4 O17 159.6(2) . . ?
O4 W4 O8 91.3(2) . . ?
O4 W4 O13 85.90(19) . . ?
O7 W4 O6 102.0(2) . . ?
O7 W4 O17 96.1(2) . . ?
O7 W4 O8 101.5(2) . . ?
O7 W4 O13 169.9(2) . . ?
O7 W4 O4 104.2(2) . . ?
O33 W5 O31 75.04(18) . . ?
O24 W5 O33 85.0(2) . . ?
O24 W5 O26 153.3(2) . . ?
O24 W5 O31 76.93(18) . . ?
O20 W5 O33 161.1(2) . . ?
O20 W5 O24 93.1(2) . . ?
O20 W5 O26 90.4(2) . . ?
O20 W5 O31 86.18(19) . . ?
O26 W5 O33 83.3(2) . . ?
O26 W5 O31 76.85(18) . . ?
O25 W5 O33 95.5(2) . . ?
O25 W5 O24 102.5(2) . . ?
O25 W5 O20 103.2(2) . . ?
O25 W5 O26 102.5(2) . . ?
O25 W5 O31 170.6(2) . . ?
O30 W6 O35 81.8(2) . . ?
O30 W6 O31 77.07(19) . . ?
O22 W6 O30 92.5(2) . . ?
O22 W6 O28 93.7(2) . . ?
O22 W6 O35 159.6(2) . . ?
O22 W6 O31 85.53(18) . . ?
O28 W6 O30 153.3(2) . . ?
O28 W6 O35 83.4(2) . . ?
O28 W6 O31 77.56(18) . . ?
O35 W6 O31 74.08(18) . . ?
O29 W6 O30 101.1(2) . . ?
O29 W6 O22 103.9(2) . . ?
O29 W6 O28 102.6(2) . . ?
O29 W6 O35 96.4(2) . . ?
O29 W6 O31 170.5(2) . . ?
O15 W8 O16 87.1(2) . . ?
O15 W8 O17 153.4(2) . . ?
O15 W8 O14 87.4(2) . . ?
O15 W8 O13 76.52(18) . . ?
O16 W8 O13 77.00(18) . . ?
O17 W8 O16 86.5(2) . . ?
O17 W8 O14 87.3(2) . . ?
O17 W8 O13 76.84(18) . . ?
O14 W8 O16 154.40(19) . . ?
O14 W8 O13 77.41(18) . . ?
O18 W8 O15 102.0(2) . . ?
O18 W8 O16 102.4(2) . . ?
O18 W8 O17 104.6(2) . . ?
O18 W8 O14 103.2(2) . . ?
O18 W8 O13 178.4(2) . . ?
O26 W9 O28 154.6(2) . . ?
O26 W9 O31 77.88(18) . . ?
O26 W9 O34 83.8(2) . . ?
O28 W9 O31 77.42(19) . . ?
O28 W9 O34 83.9(2) . . ?
O21 W9 O26 93.0(2) . . ?
O21 W9 O28 91.4(2) . . ?
O21 W9 O31 86.37(18) . . ?
O21 W9 O34 160.8(2) . . ?
O34 W9 O31 74.5(2) . . ?
O27 W9 O26 101.6(2) . . ?
O27 W9 O28 101.7(2) . . ?
O27 W9 O31 170.1(2) . . ?
O27 W9 O21 103.5(2) . . ?
O27 W9 O34 95.6(3) . . ?
O32 W10 O33 86.7(2) . . ?
O32 W10 O31 77.41(19) . . ?
O33 W10 O31 77.61(18) . . ?
O35 W10 O32 88.8(2) . . ?
O35 W10 O33 154.9(2) . . ?
O35 W10 O31 77.33(19) . . ?
O35 W10 O34 86.8(2) . . ?
O34 W10 O32 154.0(2) . . ?
O34 W10 O33 86.5(2) . . ?
O34 W10 O31 76.66(19) . . ?
O36 W10 O32 102.3(3) . . ?
O36 W10 O33 102.2(3) . . ?
O36 W10 O35 102.9(3) . . ?
O36 W10 O31 179.6(3) . . ?
O36 W10 O34 103.6(3) . . ?
O2 La1 O3 74.33(15) . . ?
O20 La1 O3 75.69(15) . . ?
O20 La1 O2 72.14(15) . . ?
O20 La1 O19 75.21(16) . . ?
O20 La1 O4 143.17(16) . . ?
O22 La1 O3 139.14(15) . . ?
O22 La1 O2 145.88(15) . . ?
O22 La1 O20 115.75(16) . . ?
O22 La1 O19 72.28(16) . . ?
O22 La1 O4 78.72(15) . . ?
O19 La1 O3 145.06(16) . . ?
O19 La1 O2 78.65(16) . . ?
O1 La1 O3 114.23(16) . . ?
O1 La1 O2 73.47(16) . . ?
O1 La1 O20 139.60(16) . . ?
O1 La1 O22 83.15(15) . . ?
O1 La1 O19 77.84(16) . . ?
O1 La1 O21 146.02(16) . . ?
O1 La1 O4 72.43(16) . . ?
O21 La1 O3 72.68(15) . . ?
O21 La1 O2 137.27(15) . . ?
O21 La1 O20 73.98(15) . . ?
O21 La1 O22 73.59(15) . . ?
O21 La1 O19 116.53(16) . . ?
O21 La1 O4 78.88(15) . . ?
O4 La1 O3 72.75(15) . . ?
O4 La1 O2 115.85(15) . . ?
O4 La1 O19 140.44(16) . . ?
W8 O15 W3 116.3(2) . . ?
W8 O16 W1 115.7(2) . . ?
W4 O6 W2 115.6(2) . . ?
W3 O10 W1 115.0(2) . . ?
W8 O17 W4 117.0(2) . . ?
W7 O30 W6 114.6(2) . . ?
W3 O12 W2 115.0(2) . . ?
W8 O14 W2 116.1(2) . . ?
W10 O32 W7 115.5(2) . . ?
W1 O3 La1 129.2(2) . . ?
W10 O33 W5 115.5(2) . . ?
W5 O24 W7 116.0(2) . . ?
W3 O2 La1 127.4(2) . . ?
W5 O20 La1 128.1(2) . . ?
W6 O22 La1 128.8(2) . . ?
W9 O26 W5 114.5(2) . . ?
W7 O19 La1 127.2(2) . . ?
W1 O8 W4 114.2(2) . . ?
W2 O1 La1 130.2(2) . . ?
W6 O28 W9 114.5(2) . . ?
W10 O35 W6 115.9(2) . . ?
Na3 O48 Na2 116.0(2) . . ?
Na4 O42 Na6 95.5(2) 2_666 . ?
W1 O13 W2 175.5(2) . . ?
W1 O13 W4 89.72(16) . . ?
W1 O13 W8 92.19(17) . . ?
W2 O13 W4 88.60(16) . . ?
W3 O13 W1 91.24(16) . . ?
W3 O13 W2 90.06(16) . . ?
W3 O13 W4 174.8(2) . . ?
W3 O13 W8 92.75(16) . . ?
W8 O13 W2 92.10(16) . . ?
W8 O13 W4 92.31(16) . . ?
Na7 O41 Na4 126.2(3) 1_554 . ?
W6 O31 W5 175.5(2) . . ?
W9 O31 W5 90.22(16) . . ?
W9 O31 W6 89.83(16) . . ?
W9 O31 W7 175.4(2) . . ?
W10 O31 W5 91.78(16) . . ?
W10 O31 W6 92.68(17) . . ?
W10 O31 W9 92.34(16) . . ?
W10 O31 W7 92.24(17) . . ?
W7 O31 W5 89.75(16) . . ?
W7 O31 W6 89.85(16) . . ?
W9 O21 La1 127.7(2) . . ?
W10 O34 W9 116.5(3) . . ?
W1 O9 Na4 137.7(3) . . ?
Na1 O53 Na2 79.58(18) . . ?
Na3 O46 Na6 125.6(2) . . ?
W4 O4 La1 128.5(2) . . ?
Na6 O43 Na7 125.0(2) . 2_667 ?
Na1 O52 Na2 82.95(19) . . ?
Na9 O62 Na5 85.3(2) . . ?
Na2 O50 Na1 82.66(18) . . ?
W2 O5 Na5 138.7(3) . . ?
W2 O5 Na9 127.4(3) . . ?
Na5 O5 Na9 77.22(19) . . ?
Na3 O39 Na4 113.8(2) . . ?
W6 O29 Na8 145.1(3) . . ?
W9 O27 Na3 145.6(3) . 2_656 ?
Na4 O44 Na6 96.8(2) 2_666 . ?
Na9 O65 Na5 83.2(2) . . ?
W7 O23 Na9 125.7(4) . 2_667 ?
Na8 O67 Na7 84.7(2) . . ?
W3 O11 Na3 134.4(3) . 2_666 ?
Na7 O58 Na8 86.0(4) . . ?
O30 W7 O32 83.5(2) . . ?
O30 W7 O24 152.9(2) . . ?
O30 W7 O31 77.30(19) . . ?
O32 W7 O31 74.78(19) . . ?
O24 W7 O32 82.3(2) . . ?
O24 W7 O31 76.77(19) . . ?
O19 W7 O30 93.8(2) . . ?
O19 W7 O32 161.5(2) . . ?
O19 W7 O24 92.4(2) . . ?
O19 W7 O31 86.73(19) . . ?
O23 W7 O30 101.6(3) . . ?
O23 W7 O32 92.7(3) . . ?
O23 W7 O24 102.0(3) . . ?
O23 W7 O19 105.8(3) . . ?
O23 W7 O31 167.4(3) . . ?
O53 Na1 O50 91.3(2) . . ?
O53 Na1 Na2 51.33(15) . . ?
O52 Na1 O53 75.4(2) . . ?
O52 Na1 O50 76.64(19) . . ?
O52 Na1 O56 89.6(2) . . ?
O52 Na1 Na2 49.37(15) . . ?
O50 Na1 Na2 46.90(14) . . ?
O56 Na1 O53 104.6(2) . . ?
O56 Na1 O50 155.8(2) . . ?
O56 Na1 Na2 133.67(18) . . ?
O54 Na1 O53 169.2(2) . . ?
O54 Na1 O52 108.4(2) . . ?
O54 Na1 O50 80.0(2) . . ?
O54 Na1 O56 85.8(2) . . ?
O54 Na1 Na2 123.2(2) . . ?
O55 Na1 O53 81.2(3) . . ?
O55 Na1 O52 152.9(3) . . ?
O55 Na1 O50 90.5(2) . . ?
O55 Na1 O56 109.7(3) . . ?
O55 Na1 O54 92.4(3) . . ?
O55 Na1 Na2 104.7(3) . . ?
O48 Na2 O53 150.2(2) . . ?
O48 Na2 Na1 118.36(17) . . ?
O48 Na2 Na3 31.43(13) . . ?
O51 Na2 O48 86.6(2) . . ?
O51 Na2 O53 123.0(2) . . ?
O51 Na2 Na1 125.98(18) . . ?
O51 Na2 Na3 117.02(17) . . ?
O53 Na2 Na1 49.09(15) . . ?
O53 Na2 Na3 118.91(16) . . ?
O49 Na2 O48 86.6(2) . . ?
O49 Na2 O51 90.9(2) . . ?
O49 Na2 O53 89.5(2) . . ?
O49 Na2 O52 108.5(2) . . ?
O49 Na2 O50 173.5(2) . . ?
O49 Na2 Na1 134.00(18) . . ?
O49 Na2 Na3 79.04(16) . . ?
O52 Na2 O48 80.4(2) . . ?
O52 Na2 O51 155.8(2) . . ?
O52 Na2 O53 72.86(19) . . ?
O52 Na2 Na1 47.68(15) . . ?
O52 Na2 Na3 55.69(15) . . ?
O50 Na2 O48 94.7(2) . . ?
O50 Na2 O51 82.9(2) . . ?
O50 Na2 O53 92.5(2) . . ?
O50 Na2 O52 77.9(2) . . ?
O50 Na2 Na1 50.44(15) . . ?
O50 Na2 Na3 105.30(16) . . ?
Na1 Na2 Na3 102.12(10) . . ?
O48 Na3 O38 111.5(2) . . ?
O48 Na3 O46 85.8(2) . . ?
O48 Na3 O27 75.23(19) . 2_656 ?
O48 Na3 O11 140.2(2) . 2_666 ?
O48 Na3 Na2 32.60(14) . . ?
O48 Na3 Na4 125.98(17) . . ?
O38 Na3 O46 82.9(2) . . ?
O38 Na3 O27 155.7(2) . 2_656 ?
O38 Na3 Na2 126.46(17) . . ?
O38 Na3 Na4 78.95(15) . . ?
O46 Na3 O27 121.4(2) . 2_656 ?
O46 Na3 Na2 63.43(14) . . ?
O46 Na3 Na4 147.44(17) . . ?
O39 Na3 O48 92.8(2) . . ?
O39 Na3 O38 88.1(2) . . ?
O39 Na3 O46 169.6(2) . . ?
O39 Na3 O27 67.95(18) . 2_656 ?
O39 Na3 O11 97.7(2) . 2_666 ?
O39 Na3 Na2 119.23(17) . . ?
O39 Na3 Na4 33.28(14) . . ?
O27 Na3 Na2 72.17(14) 2_656 . ?
O27 Na3 Na4 78.56(14) 2_656 . ?
O11 Na3 O38 107.1(2) 2_666 . ?
O11 Na3 O46 89.88(19) 2_666 . ?
O11 Na3 O27 73.55(18) 2_666 2_656 ?
O11 Na3 Na2 112.72(16) 2_666 . ?
O11 Na3 Na4 70.31(14) 2_666 . ?
Na4 Na3 Na2 147.71(11) . . ?
O40 Na4 O42 171.0(2) . 2_666 ?
O40 Na4 O41 95.6(2) . . ?
O40 Na4 O9 85.81(19) . . ?
O40 Na4 Na3 114.67(16) . . ?
O40 Na4 Na6 134.04(17) . 2_666 ?
O42 Na4 O41 93.0(2) 2_666 . ?
O42 Na4 O9 85.87(19) 2_666 . ?
O42 Na4 Na3 70.87(15) 2_666 . ?
O42 Na4 Na6 42.46(15) 2_666 2_666 ?
O41 Na4 O9 175.9(2) . . ?
O41 Na4 Na3 72.05(15) . . ?
O41 Na4 Na6 91.79(16) . 2_666 ?
O9 Na4 Na3 103.82(15) . . ?
O9 Na4 Na6 90.04(15) . 2_666 ?
O39 Na4 O40 83.4(2) . . ?
O39 Na4 O42 100.5(2) . 2_666 ?
O39 Na4 O41 83.9(2) . . ?
O39 Na4 O9 92.3(2) . . ?
O39 Na4 Na3 32.88(14) . . ?
O39 Na4 Na6 142.55(18) . 2_666 ?
O44 Na4 O40 92.6(2) 2_666 . ?
O44 Na4 O42 84.2(2) 2_666 2_666 ?
O44 Na4 O41 92.2(2) 2_666 . ?
O44 Na4 O9 91.7(2) 2_666 . ?
O44 Na4 O39 174.1(2) 2_666 . ?
O44 Na4 Na3 149.22(18) 2_666 . ?
O44 Na4 Na6 41.76(16) 2_666 2_666 ?
Na6 Na4 Na3 110.77(11) 2_666 . ?
O62 Na5 O5 90.6(2) . . ?
O62 Na5 O65 78.2(2) . . ?
O62 Na5 O60 80.7(2) . . ?
O62 Na5 Na9 46.97(18) . . ?
O5 Na5 Na9 52.30(16) . . ?
O61 Na5 O62 98.2(2) . . ?
O61 Na5 O5 150.8(2) . . ?
O61 Na5 O65 80.0(2) . . ?
O61 Na5 O60 105.5(3) . . ?
O61 Na5 Na9 117.3(2) . . ?
O65 Na5 O5 74.7(2) . . ?
O65 Na5 O60 158.7(3) . . ?
O65 Na5 Na9 47.88(19) . . ?
O59 Na5 O62 165.5(3) . . ?
O59 Na5 O5 82.2(2) . . ?
O59 Na5 O61 94.1(2) . . ?
O59 Na5 O65 111.7(2) . . ?
O59 Na5 O60 88.6(2) . . ?
O59 Na5 Na9 131.9(2) . . ?
O60 Na5 O5 103.3(3) . . ?
O60 Na5 Na9 113.9(2) . . ?
O42 Na6 O46 77.1(2) . . ?
O42 Na6 O43 83.4(2) . . ?
O42 Na6 O45 104.1(2) . . ?
O42 Na6 Na4 42.00(15) . 2_666 ?
O46 Na6 O43 127.3(2) . . ?
O46 Na6 O45 77.6(2) . . ?
O46 Na6 Na4 110.81(17) . 2_666 ?
O43 Na6 O45 155.2(2) . . ?
O43 Na6 Na4 82.67(17) . 2_666 ?
O45 Na6 Na4 87.40(17) . 2_666 ?
O44 Na6 O42 83.4(2) . . ?
O44 Na6 O46 136.2(2) . . ?
O44 Na6 O43 88.1(2) . . ?
O44 Na6 O45 69.7(2) . . ?
O44 Na6 Na4 41.42(15) . 2_666 ?
O47 Na6 O42 171.8(3) . . ?
O47 Na6 O46 108.7(2) . . ?
O47 Na6 O43 88.4(2) . . ?
O47 Na6 O45 83.0(2) . . ?
O47 Na6 O44 95.6(2) . . ?
O47 Na6 Na4 136.1(2) . 2_666 ?
O41 Na7 O43 84.4(2) 1_556 2_667 ?
O41 Na7 O67 98.2(2) 1_556 . ?
O41 Na7 O68B 158.3(3) 1_556 . ?
O41 Na7 Na8 126.8(2) 1_556 . ?
O43 Na7 Na8 134.8(2) 2_667 . ?
O57 Na7 O41 117.6(3) . 1_556 ?
O57 Na7 O43 91.0(2) . 2_667 ?
O57 Na7 O67 83.1(2) . . ?
O57 Na7 O68B 84.1(3) . . ?
O57 Na7 O58 151.1(5) . . ?
O57 Na7 Na8 98.9(2) . . ?
O67 Na7 O43 174.1(2) . 2_667 ?
O67 Na7 Na8 47.00(17) . . ?
O58 Na7 O41 84.3(4) . 1_556 ?
O58 Na7 O43 110.8(4) . 2_667 ?
O58 Na7 O67 74.8(4) . . ?
O58 Na7 O68B 75.1(4) . . ?
O58 Na7 Na8 52.3(4) . . ?
O66 Na8 O67 106.4(3) . . ?
O66 Na8 O70 81.8(3) . . ?
O66 Na8 O58 71.6(3) . . ?
O66 Na8 O69A 163.5(6) . . ?
O66 Na8 Na7 112.3(2) . . ?
O29 Na8 O66 106.7(3) . . ?
O29 Na8 O67 82.2(2) . . ?
O29 Na8 O70 96.3(3) . . ?
O29 Na8 O58 148.3(3) . . ?
O29 Na8 O68A 153.3(5) . . ?
O29 Na8 O69A 75.8(5) . . ?
O29 Na8 Na7 123.1(2) . . ?
O67 Na8 O58 68.7(3) . . ?
O67 Na8 O69A 90.0(6) . . ?
O67 Na8 Na7 48.28(18) . . ?
O70 Na8 O67 171.7(3) . . ?
O70 Na8 O58 114.3(3) . . ?
O70 Na8 O69A 81.8(6) . . ?
O70 Na8 Na7 128.3(2) . . ?
O58 Na8 Na7 41.7(3) . . ?
O62 Na9 O5 89.7(2) . . ?
O62 Na9 O65 79.5(3) . . ?
O62 Na9 O23 95.6(3) . 2_667 ?
O62 Na9 Na5 47.71(18) . . ?
O5 Na9 O23 149.6(2) . 2_667 ?
O5 Na9 Na5 50.48(15) . . ?
O65 Na9 O5 74.2(2) . . ?
O65 Na9 O23 77.5(2) . 2_667 ?
O65 Na9 Na5 48.93(18) . . ?
O23 Na9 Na5 114.9(2) 2_667 . ?
O63 Na9 O62 80.6(3) . . ?
O63 Na9 O5 79.6(3) . . ?
O63 Na9 O65 146.9(3) . . ?
O63 Na9 O23 130.8(3) . 2_667 ?
O63 Na9 Na5 98.5(3) . . ?
O64 Na9 O62 173.2(4) . . ?
O64 Na9 O5 90.8(3) . . ?
O64 Na9 O65 94.1(3) . . ?
O64 Na9 O23 80.6(3) . 2_667 ?
O64 Na9 O63 106.2(3) . . ?
O64 Na9 Na5 128.9(3) . . ?
O58 O68Ab Na7 72.4(8) . . ?
O58 O68Ab Na8 82.4(8) . . ?
Na7 O68Ab Na8 100.4(6) . . ?
Na8 O68Ba Na7 93.6(4) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O16 2.024(5) . ?
W1 O10 1.969(4) . ?
W1 O3 1.786(5) . ?
W1 O8 1.939(4) . ?
W1 O13 2.312(5) . ?
W1 O9 1.742(5) . ?
O68Ba Na7 2.422(10) . ?
O68Ab Na7 2.126(19) . ?
O68Ba Na8 2.312(11) . ?
O69Ab Na8 2.62(2) . ?
O68Ab Na8 2.364(16) . ?
W2 O6 1.958(4) . ?
W2 O12 1.951(5) . ?
W2 O14 2.042(4) . ?
W2 O1 1.787(5) . ?
W2 O13 2.344(5) . ?
W2 O5 1.731(5) . ?
W3 O15 2.034(4) . ?
W3 O10 1.943(5) . ?
W3 O12 1.949(5) . ?
W3 O2 1.785(5) . ?
W3 O13 2.306(5) . ?
W3 O11 1.736(5) . ?
W4 O6 1.912(5) . ?
W4 O17 2.038(5) . ?
W4 O8 1.973(5) . ?
W4 O13 2.345(5) . ?
W4 O4 1.801(5) . ?
W4 O7 1.733(5) . ?
W5 O33 2.023(5) . ?
W5 O24 1.927(5) . ?
W5 O20 1.783(5) . ?
W5 O26 1.972(5) . ?
W5 O31 2.335(5) . ?
W5 O25 1.743(5) . ?
W6 O30 1.957(5) . ?
W6 O22 1.782(5) . ?
W6 O28 1.936(5) . ?
W6 O35 2.055(5) . ?
W6 O31 2.327(5) . ?
W6 O29 1.744(5) . ?
W8 O15 1.903(5) . ?
W8 O16 1.914(5) . ?
W8 O17 1.904(5) . ?
W8 O14 1.911(5) . ?
W8 O13 2.316(5) . ?
W8 O18 1.734(5) . ?
W9 O26 1.944(5) . ?
W9 O28 1.960(5) . ?
W9 O31 2.314(5) . ?
W9 O21 1.796(4) . ?
W9 O34 2.017(5) . ?
W9 O27 1.732(5) . ?
W10 O32 1.912(6) . ?
W10 O33 1.917(5) . ?
W10 O35 1.900(5) . ?
W10 O31 2.308(5) . ?
W10 O34 1.903(6) . ?
W10 O36 1.742(6) . ?
La1 O3 2.530(5) . ?
La1 O2 2.527(4) . ?
La1 O20 2.518(5) . ?
La1 O22 2.516(5) . ?
La1 O19 2.520(5) . ?
La1 O1 2.501(5) . ?
La1 O21 2.507(5) . ?
La1 O4 2.520(5) . ?
O30 W7 1.947(5) . ?
O32 W7 2.035(5) . ?
O24 W7 1.949(5) . ?
O19 W7 1.794(5) . ?
O40 Na4 2.401(6) . ?
O48 Na2 2.465(6) . ?
O48 Na3 2.386(6) . ?
O42 Na4 2.411(6) 2_666 ?
O42 Na6 2.433(6) . ?
O38 Na3 2.428(6) . ?
O41 Na4 2.421(6) . ?
O41 Na7 2.357(6) 1_554 ?
O31 W7 2.325(5) . ?
O51 Na2 2.453(6) . ?
O9 Na4 2.522(6) . ?
O53 Na1 2.452(6) . ?
O53 Na2 2.533(6) . ?
O46 Na3 2.444(6) . ?
O46 Na6 2.493(6) . ?
O49 Na2 2.326(6) . ?
O43 Na6 2.510(7) . ?
O43 Na7 2.621(7) 2_667 ?
O52 Na1 2.377(6) . ?
O52 Na2 2.440(6) . ?
O62 Na5 2.377(7) . ?
O62 Na9 2.349(8) . ?
O50 Na1 2.481(6) . ?
O50 Na2 2.349(6) . ?
O57 Na7 2.284(7) . ?
O5 Na5 2.533(6) . ?
O5 Na9 2.598(7) . ?
O56 Na1 2.381(6) . ?
O39 Na3 2.369(6) . ?
O39 Na4 2.394(6) . ?
O66 Na8 2.371(9) . ?
O45 Na6 2.570(7) . ?
O29 Na8 2.356(7) . ?
O27 Na3 2.992(7) 2_656 ?
O44 Na4 2.390(6) 2_666 ?
O44 Na6 2.406(7) . ?
O54 Na1 2.365(7) . ?
O55 Na1 2.274(7) . ?
O47 Na6 2.365(7) . ?
O61 Na5 2.355(7) . ?
O65 Na5 2.432(7) . ?
O65 Na9 2.392(8) . ?
O59 Na5 2.351(6) . ?
O23 W7 1.717(6) . ?
O23 Na9 2.906(9) 2_667 ?
O63 Na9 2.326(9) . ?
O60 Na5 2.446(8) . ?
O67 Na7 2.587(8) . ?
O67 Na8 2.535(8) . ?
O70 Na8 2.419(9) . ?
O64 Na9 2.316(9) . ?
O11 Na3 2.419(6) 2_666 ?
O58 O68A 1.73(2) . ?
O58 Na7 2.302(12) . ?
O58 Na8 2.738(15) . ?
Na1 Na2 3.191(4) . ?
Na2 Na3 4.114(4) . ?
Na3 O27 2.992(7) 2_656 ?
Na3 O11 2.419(6) 2_666 ?
Na3 Na4 3.991(4) . ?
Na4 O42 2.411(6) 2_666 ?
Na4 O44 2.390(6) 2_666 ?
Na4 Na6 3.587(5) 2_666 ?
Na5 Na9 3.203(6) . ?
Na6 Na4 3.587(5) 2_666 ?
Na7 O41 2.357(6) 1_556 ?
Na7 O43 2.621(7) 2_667 ?
Na7 Na8 3.452(6) . ?
Na9 O23 2.906(9) 2_667 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
La1 O19 W7 O30 78.2(3) . . . . ?
La1 O19 W7 O32 -2.8(9) . . . . ?
La1 O19 W7 O24 -75.4(3) . . . . ?
La1 O19 W7 O31 1.2(3) . . . . ?
La1 O19 W7 O23 -178.6(3) . . . . ?
O15 W3 O2 La1 -6.8(8) . . . . ?
O15 W3 O11 Na3 31.6(4) . . . 2_666 ?
O16 W1 O3 La1 -6.1(8) . . . . ?
O16 W1 O9 Na4 -99.5(4) . . . . ?
O6 W2 O1 La1 -78.9(3) . . . . ?
O6 W2 O5 Na5 175.6(4) . . . . ?
O6 W2 O5 Na9 -67.9(3) . . . . ?
O6 W4 O4 La1 75.5(3) . . . . ?
O10 W1 O3 La1 -77.4(3) . . . . ?
O10 W1 O9 Na4 -15.3(4) . . . . ?
O10 W3 O2 La1 74.7(3) . . . . ?
O10 W3 O11 Na3 -52.6(4) . . . 2_666 ?
O17 W4 O4 La1 -7.9(8) . . . . ?
O30 W6 O22 La1 -79.2(3) . . . . ?
O30 W6 O29 Na8 -53.6(6) . . . . ?
O12 W2 O1 La1 74.1(3) . . . . ?
O12 W2 O5 Na5 7.0(4) . . . . ?
O12 W2 O5 Na9 123.5(3) . . . . ?
O12 W3 O2 La1 -79.4(3) . . . . ?
O12 W3 O11 Na3 115.5(4) . . . 2_666 ?
O14 W2 O1 La1 -5.8(8) . . . . ?
O14 W2 O5 Na5 91.6(4) . . . . ?
O14 W2 O5 Na9 -151.8(3) . . . . ?
O3 W1 O9 Na4 78.3(4) . . . . ?
O33 W5 O20 La1 -9.2(9) . . . . ?
O24 W5 O20 La1 74.4(3) . . . . ?
O2 W3 O11 Na3 -149.6(3) . . . 2_666 ?
O22 W6 O29 Na8 41.8(6) . . . . ?
O26 W5 O20 La1 -79.1(3) . . . . ?
O26 W9 O21 La1 75.6(3) . . . . ?
O26 W9 O27 Na3 2.1(6) . . . 2_656 ?
O8 W1 O3 La1 76.9(3) . . . . ?
O8 W1 O9 Na4 174.2(3) . . . . ?
O8 W4 O4 La1 -78.9(3) . . . . ?
O1 W2 O5 Na5 -89.5(4) . . . . ?
O1 W2 O5 Na9 27.0(4) . . . . ?
O28 W6 O22 La1 74.8(3) . . . . ?
O28 W6 O29 Na8 138.9(5) . . . . ?
O28 W9 O21 La1 -79.4(3) . . . . ?
O28 W9 O27 Na3 171.9(5) . . . 2_656 ?
O35 W6 O22 La1 -6.2(8) . . . . ?
O35 W6 O29 Na8 -136.4(5) . . . . ?
O13 W1 O3 La1 -1.3(3) . . . . ?
O13 W2 O1 La1 -2.1(3) . . . . ?
O13 W3 O2 La1 -2.0(3) . . . . ?
O13 W3 O11 Na3 24.9(13) . . . 2_666 ?
O13 W4 O4 La1 -2.0(3) . . . . ?
O31 W5 O20 La1 -2.3(3) . . . . ?
O31 W6 O22 La1 -2.4(3) . . . . ?
O31 W9 O21 La1 -2.1(3) . . . . ?
O21 W9 O27 Na3 -93.8(5) . . . 2_656 ?
O34 W9 O21 La1 -4.1(8) . . . . ?
O34 W9 O27 Na3 87.0(5) . . . 2_656 ?
O9 W1 O3 La1 -179.4(3) . . . . ?
O5 W2 O1 La1 177.4(3) . . . . ?
O7 W4 O4 La1 178.9(3) . . . . ?
O25 W5 O20 La1 178.0(3) . . . . ?
O29 W6 O22 La1 178.7(3) . . . . ?
O27 W9 O21 La1 178.3(3) . . . . ?
O11 W3 O2 La1 177.0(3) . . . . ?
Na7 O58 O68Ab Na8 -103.5(5) . . . . ?
Na9 O23 W7 O30 -56.3(4) 2_667 . . . ?
Na9 O23 W7 O32 27.7(4) 2_667 . . . ?
Na9 O23 W7 O24 110.3(4) 2_667 . . . ?
Na9 O23 W7 O19 -153.7(3) 2_667 . . . ?
Na9 O23 W7 O31 27.3(14) 2_667 . . . ?
Na8 O58 O68Ab Na7 103.5(5) . . . . ?
